bluuebunny/crossref_metadata_2025_split huggingface dataset:
Investigation of Worn Chain Links
Authors: Naumann Friedrich Karl , Spies Ferdinand 
Published: May 2019

Abstract
Three links of a chain showing unusually strong wear were examined. Corresponding to the stress, the wear was strongest in the bends of the links, but it was especially pronounced in the bend in which the butt weld seam was located. Investigation showed the links were manufactured from an unkilled carbon-deficient steel, and were case hardened to a depth of 0.8 to 0.9 mm. The peripheral structure at the places not showing wear consisted of coarse acicular martensite with a high percentage of retained austenite. The links therefore were strongly overheated, probably directly heated during case hardening. The butt weld seams were not tight and were covered with oxide inclusions. Given that wear occurred preferentially at the welds it may be concluded that this weld defect contributed to the substantial wear. This leaves unanswered whether these chains could have withstood the high operating stress if they had been welded satisfactorily and hardened correctly, and whether it made any sense to case harden highly stressed chains of this type.
Fractures of Flat Wire Conveyor Belt Links of Glass Annealing Furnaces
Authors: Naumann Friedrich Karl , Spies Ferdinand 
Published: May 2019

Abstract
The cross bars of conveyor belt links that served to transport glass containers through a stress relief furnace fractured in many cases. They consisted of wires of 5 mm diam made of low-carbon Siemens-Martin steel, while the interwoven longitudinal bars were made of strip steel of 4 x 2 sq mm. The furnace temperature was said to be 500 deg C. In addition to the fractures they also showed many more or less advanced cracks. These occurred in the circumferential grooves that recurred at regular intervals. The fractures were abraded and oxidized. They could have been fatigue fractures. The fracture probably was induced by the pressing-in or abrading of the sharp steel band edges into the surface of the cross bars. Torsion fatigue fractures may have started from these notches. Relaxation then contributed positively through recovery and recrystallization. Such damage occurs less frequently in round wire conveyor belt links because the round wire neither impresses so sharply nor abrades against the cross bars, and it also exerts less torsion than the flat wire.
Failure Analysis of Wire Rope
Authors: Miller Brett A. 
Published: May 2019

Abstract
Mechanical properties of wire ropes, their chemical composition, and the failure analysis process for them are described. The wires are manufactured from high-carbon, plain carbon steel, with high-strength ropes most often manufactured from AISI Grade 1074. During visual failure examination, the rope, strand, and wire diameters should all be measured. Examination should also address the presence or absence of lubricant, corrosion evidence, and gross mechanical damage. Failed wires can exhibit classic cup-and-cone ductile features, flat fatigue features, and various appearances in-between. However, wires are often mechanically damaged after failure. Most nondestructive evaluation (NDE) techniques are not applicable to wire rope failures. Electron microscope fractography of fracture surfaces is essential in failure analysis. Fatigue is the most important fracture mode in wire ropes. Metallographic features of wire ropes that failed because of ductile overload and fatigue are described.
An Analysis of Six Fatigue Failures in Cranes
Authors: Williams W. M. , Firth Mark 
Published: May 2019

Abstract
Crane collapse due to bolt fatigue and fatigue failure of a crane support column, crane tower, overhead yard crane, hoist rope, and overhead crane drive shaft are described. The first four examples relate to the structural integrity of cranes. However, equipment such as drive and hoist-train components are often subject to severe fatigue loading and are perhaps even more prone to fatigue failure. In all instances, the presence of fatigue cracks at least contributed to the failure. In most instances, fatigue was the sole cause. Further, in each case, with regular inspection, fatigue cracks probably would have been detected well before final failure.
Fractured Valve Spring
Authors: Naumann Friedrich Karl , Spies Ferdinand 
Published: May 2019

Abstract
A steel valve spring meeting Steel-Iron-Test 1570 fractured during the high-stress condition of the operation of its valve. Metallographic examination of a transverse section adjacent to the fracture and a longitudinal section through the crack showed the steel was free of major defects and was of high purity, although a number of minor surface defects such as rolling laps were found. The spring was heat treated and its surface strengthened by shot-peening, but the surface was also decarburized to a depth of approximately 0.03 mm which resulted in a lowering of the surface hardness. The fracture of this valve spring is therefore primarily due to surface defects, and secondly perhaps also to weak surface decarburization. No recommendation resulted from the investigation except to note that comparatively minor effects suffice to cause fractures in highly stressed springs.
Broken Full Lift Disk of a Safety Valve
Authors: Kauczor Egon 
Published: May 2019

Abstract
A full lift disk, made of die cast brass, which served as a lifting aid in a safety valve, had cracked in service at a number of locations in the vicinity of the threaded hole. During microscopic examination, agglomeration of oxide inclusions were noted in the region of the cracks. Because the die cast brass was alloyed with aluminum, these inclusions consisted predominantly of aluminum oxide. The tolerable limit in pores and oxide inclusions was greatly exceeded in the lift disk under examination. Above all, the numerous oxide skins disrupted the cohesion of the microstructure and were primarily responsible for the failure of the lift disk.
Destroyed Needle Bearing of a Packing Machine
Authors: Naumann Friedrich Karl , Spies Ferdinand 
Published: May 2019

Abstract
A needle bearing from a filling and seating machine for milk cartons became unusable due to corrosion and fracture of a ring after only four weeks of operation of the machine in a Finnish milk packing plant. These bearings were subject to corrosion by water condensates in this type of environment because of constant temperature changes, and they normally are replaced after eight months. The bearings were lubricated by a molybdenum sulfide paste. Judging by their structure the needles probably consisted of ball bearing steel. They showed corroded initial cracks of the pitting type, i.e., shear-fatigue fractures due to excessive surface pressure. The needles too were overstressed by compression. It seemed that the higher pressure necessary for the pressing of thicker paper accelerated the corrosion, which lead to the crack initiations of the parts and possibly also to impaired lubrication. The machine manufacturer therefore switched to bearings with shells of a complex bronze.
A Survey of the Causes of Failure of Rolling Bearings
Authors: Hutchings F.R. 
Published: May 2019

Abstract
Factors which may lead to premature roller bearing failure in service include incorrect fitting, excessive pre-load during installation, insufficient or unsuitable lubrication, over-load, impact load vibration, excessive temperature, contamination by abrasive matter, ingress of harmful liquids, and stray electric currents. Most common modes of failure include flaking or pitting (fatigue), cracks or fractures, creep, smearing, wear, softening, indentation, fluting, and corrosion. The modes of failure are illustrated with examples from practice.
Wear Failure of a Leaded Bronze Bearing: Correlation Between Plant Experience and Laboratory Wear Test Data
Authors: Ahsan Q. , Haseeb A.S.M.A. , Haque E. , Celis J.P. 
Published: May 2019

Abstract
This paper describes an investigation on the failure of a large leaded bronze bearing that supports a nine-ton roller of a plastic calendering machine. At the end of the normal service life of a good bearing, which lasted for seven years, a new bearing was installed. However the new one failed catastrophically within a few days, generating a huge amount of metallic wear debris and causing pitting on the surface of the cast iron roller. Following the failure, samples were collected from both good and failed bearings. The samples were analyzed chemically and their microstructures examined. Both samples were subjected to accelerated wear tests in a laboratory type pin-on-disk apparatus. During the tests, the bearing materials acted as pins, which were pressed against a rotating cast iron disk. The wear behaviors of both bearing materials were studied using weight loss measurement. The worn surfaces of samples and the wear debris were examined by light optical microscope, SEM, and energy-dispersive x-ray microanalyzer. It was found that the laboratory pin-on-disk wear data correlated well with the plant experience. It is suggested that the higher lead content ~18%) of the good bearing compared with 7% lead of the failed bearing helped to establish a protective transfer layer on the worn surface. This transfer layer reduced metal-to-metal contact between the bearing and the roller and resulted in a lower wear rate. The lower lead content of the failed bearing does not allow the establishment of a well-protected transfer layer and leads to rapid wear.
Failure Analysis of Helical Suspension Springs under Compressor Start/Stop Conditions
Authors: Zaccone M.A. 
Published: May 2019

Abstract
During testing of compressors under start/stop conditions, several helical suspension springs failed. The ensuing failure investigation showed that the springs failed due to fatigue. The analysis showed that during start/stop testing the springs would undergo both a lateral and axial deflection, greatly increasing the torsional stresses on the spring. To understand the fatigue limits under these test conditions, a bench test was used to establish the fatigue strength of the springs. The bench tests showed that the failed springs had an unacceptable surface texture that reduced the fatigue life. Based on an understanding of the compressor motion, a Monte Carlo model was developed based on a linear damage theory to predict the fatigue life of the springs during start/stop conditions. The results of this model were compared to actual test data. The model showed that the design was marginal even for springs with acceptable surface texture. The model was then used to predict the fatigue life requirements on the bench test such that the reliability goals for the start/stop testing would be met, thus reducing the risk in qualifying the compressor.
Microstructural Analysis of the Brass Seat of a Valve from the 1907 Steam Tug ‘Hercules’
Authors: Brooks Charlie R. , Monday Dean 
Published: May 2019

Abstract
The steam tug Hercules was an ocean-going and bay tug for 55 years before being retired. It is now being restored by the National Park Service. A broken steam valve was obtained for microstructural examination. The body was gray cast iron, and the stem and seat were brass. The examination centered on corrosion of the brass components. The seat and shaft were alpha brass, with a hardness of 64 and 79 DPH, respectively. A nut held the shaft onto the seat, and was alpha-beta brass with a hardness of 197 DPH. Welded on the end of the shaft was a ring of hard (DPH 294) alpha-beta brass, which seated against the nut. The brass seat and stem show little corrosion. However, the alpha-beta brass nut and welded tip showed extensive dezincification. This process of removal of Zn and the retention of Cu began in the high Zn beta phase, but eventually both phases were attacked. The depth of penetration was consistent with dezincification rates reported in the literature for such brasses in salt water if the valve had been in service about 55 years.
Metallographic Characterization of Stress Corrosion Cracking in High Strength Bolts
Authors: Magner S.H. , Weins W.N. 
Published: May 2019

Abstract
Diagnosis of environmentally induced failures is greatly facilitated by metallographic analysis. As an example, a failure analysis of ASTM A574 material grade bolts is presented. The bolts served as bonnet screws in underground valves and failed due to stress-corrosion cracking. Metallographic methods were used to diagnose and provide solutions for the service failure. Included are photos showing crack propagation morphology and fracture surface appearance.
Failure of 17-4 PH Stainless Steel Bolts on a Titan Space Launch Vehicle
Authors: Raymond Louis , Kendall Ernest G. 
Published: May 2019

Abstract
Several stainless steel bolts used on a Titan Space Launch Vehicle broke at the shank and failure was attributed to stress-corrosion cracking. But results could not be duplicated in the laboratory with salt-solution immersion tests until the real culprit was established: the secondary effect of galvanic coupling, hydrogen embrittlement.
Fractography of Steel Drive Cables
Authors: Shemenski R. M. 
Published: May 2019

Abstract
Drive cables from a rubber processing machine were failing in less than 8 h of operation, the expected service life being much greater than 100 h. Comparison cables were tested to failure under known stress conditions, including tensile overload, torsional loading, reversed bending alternating stress, and buckling (compressive) cyclic loading. The mode of failure was found to be reversed bending fatigue caused by drive cables moving over guide pulleys of small radii. Modifications of the machinery and drive cable system were suggested.
Failure of Electric Motor Ball Bearing
Authors: Walton H.W. 
Published: May 2019

Abstract
Incorrect grounding of an electric motor resulted in electric current passing through a 52100 steel ball bearing and caused multiple arcing between the rolling elements. The multiple arcing developed a pattern on the outer race known as ‘fluting’. A section of ball race outer showed the distinct banding (fluting) resulting from spark discharges while the bearing was rotating. The severe distress of the surface resulted in unacceptable levels of vibration. An SEM photograph of the banded regions showed smoothing of the asperities from continued operation is evident. In the craters the residue of partial melting was seen.
Stress-Corrosion Cracking of a Brass Radiator Coil
Authors: Ogden Paul 
Published: May 2019

Abstract
An interstage radiator gas coil began leaking after only 45 days of service. The original brass coil with several aluminum fins was replaced three times but each replacement lasted less than a day. After removing the fins, leaks were found at circumferential cracks. A section of a tube was removed and split, revealing a series of cracks, evenly spaced. Crack spacing coincided with fin spacing, indicating that stresses incurred during installation of the fins promoted failure. Metallographic examination showed intergranular, branched cracking, characteristic of stress corrosion failures, with the cracks starting on the inside surfaces of the tubes. There was no known corrosive agent in the system, and no other corrosion damage could be found. Qualitative tests and spectrographic analysis gave a positive indication for mercury. The spacing of the cracks, the branched intergranular cracking, the rapid failure, and presence of mercury led to the conclusion of stress-corrosion cracking. It was impossible to remove mercury from the system so carbon steel coils were substituted for the brass ones. The carbon steel coils gave failure-free service for over nine years.
Corrosion-Erosion of a Carbon Steel Choke Body
Authors: Ogden Paul 
Published: May 2019

Abstract
A wall section of a carbon steel choke body in gas service at 4400 psig blew out three months after the use of a corrosion inhibitor was stopped. Corrosion damage occurred in ripples, leaving both smoothly polished and unattacked areas. The corrodent in condensate wells was principally carbon dioxide dissolved in water condensed from the gas stream, with organic acids possibly an aggravating factor. A gas analysis showed no other corrosive agents. No metallurgical or fabrication defects were found in the carbon steel part. The mode of attack was corrosion-erosion, caused by the corrosive, high velocity gas flow. The corrosion rate of either the inhibited or uninhibited gas stream was too high for equipment in high pressure gas service. Type 410 (12% Cr) stainless steel was recommended for the choke bodies because other equipment such as valves made of type 410 showed no evidence of corrosion damage after three years' exposure. This change was made five years ago and there have been no failures since.
Stress Corrosion Cracking Failures in Components Made of Austenitic Chromium Nickel Steels
Authors: Kauczor Egon 
Published: May 2019

Abstract
Practical examples of stress-corrosion cracking (SCC) and methods for its prevention were presented. Cracks in chloride-sensitive austenitic steels were very branched and transcrystalline. Etched cross sections of molybdenum-free samples showed chloride-induced cracks running out of the pitted areas. Alternatively polishing and etching micro-sections for viewing at high magnification made crack detail more visible. Optical and scanning electron micrographs showed cracking in austenitic cast steel and cast iron due to both internal tensile and critical residual stresses; the latter causes flake-like spalling. Measures to prevent SCC include stress reduction, use of austenitic steels or nickel alloys not susceptible to grain boundary attack, use of ferritic chromium steels, surface slag removal, control of temperature and chloride concentration, and cathodic protection.
Steel Wire Cracked at Welded Joint
Authors: Naumann Friedrich Karl , Spies Ferdinand 
Published: May 2019

Abstract
A 2.3 mm diam steel wire broke during cable twisting. The fracture occurred obliquely to the longitudinal axis of the wire and showed a constriction at the end. Therefore it was a ductile fracture. File mark type work defects were noticeable on the wire surface at both sides of the fracture, but they had no effect on the breakage of the wire. Away from the fracture area, the wire had a normal structure of hyperfine lamellar pearlite (sorbite) of a “patented” and cold drawn steel wire. In the vicinity of the fracture, the cementite of the pearlite was partially spheroidized, while at the fracture itself it was completely spheroidized. Therefore the wire was locally annealed at this point. It was likely that the wire cracked at this point during the last drawing and then broke during twisting due to its lower strength in the weakened cross section after prior deformation.
Damaged Impellers in a Rotary Pump
Authors: Kauczor Egon 
Published: May 2019

Abstract
Two damaged impellers made of austenitic cast iron came from a rotary pump used for pumping brine mixed with drifting sand. On one of the impellers, pieces were broken out of the back wall in four places at the junction to the blades. The fracture edges followed the shape of the blade. Numerous cavitation pits were seen on the inner side of the front wall visible through the breaks in the back wall. The back wall of the as yet intact second impeller which did not show such deep cavitation pits was cracked in places along the line of the blades. The microstructure consisted of lamellar graphite and carbides in an austenitic matrix and was considered normal for the specified material GGL Ni-Cu-Cr 15 6 2. It was concluded that the cause of the damage was porosity at the junction between back wall and blades arising during the casting process. Cavitation did not contribute to fracture but also could have led to damage in the long term in the case of a sound casting. It is therefore advisable in the manufacture of new impellers to take care not only to avoid porosity but also to use alloy GGL Ni-Cu-Cr 15 6 3, which has a higher chromium content and is more resistant to cavitation.
Failure Analysis of Computer Data Storage Disc Drive Systems
Authors: Tripathi K.C. 
Published: May 2019

Abstract
This paper deals with disk drive failures that occur in the interface area between the head and disk. The failures often lead to the loss of stored data and are characterized by circumferential microscratches that are usually visible to the unaided eye. The recording media in disk drives consists of a metal, glass, ceramic, or plastic substrate coated with a magnetic material. Data errors are classified as ‘soft’ or ‘hard’ depending on their correctability. Examination has shown that hard errors are the result of an abrasive wear process that begins with contact between head and disk asperities. The contact generates debris that, as it accumulates, increases contact pressure between the read-write head and the surface of the disk. Under sufficient pressure, the magnetic coating material begins wearing away, resulting in data loss.
Electron Fractography Pinpoints Cause of Fatigue Fracture
Authors: Lauchner Edward A. , Herfert Robert E. 
Published: May 2019

Abstract
After completing a fatigue test of an aluminum alloy component machined from a 7079-T6 forging, technicians noted a 5 in. crack which ran longitudinally above and through the flange. When the fracture face was examined by light microscopy, observers could not ascertain the exact mode of fracture. Electron fractography revealed that five different modes of crack growth were operative as the part failed. Region 1 was a shallow zone (about 0.002 in. at its deepest) of dimpled structure typical of an overload failure. Region 2 was a zone that grew by a stress corrosion mechanism. Through a fatigue mechanism was operative in Region 3, it was not the cause of the large crack. Region 4, which covered 50% of the fracture area, developed mainly by stress corrosion. This zone gradually changed into the combination of intergranular and transgranular overload in Region 5, which covered approximately the remaining 50% of the fracture. Apparently, after stress corrosion moved halfway through, the part failed by overload. This failure analysis proved that a crack, originally thought to be a fatigue failure, was actually a stress corrosion crack.
Cracking of Machined End Frame Steel Forgings After Heat Treatment
Authors: Das A. K. , Thippeswamy B. M. , Prasad J. 
Published: May 2019

Abstract
A number of machined end frame steel forgings made of Cr-Si-Mn alloy showed tiny cracks during magnetic particle inspection after heat treatment. The cracks were mostly confined to base edges and fillet radius. No significant abnormality was observed in chemical composition and microstructure. SEM, optical microscopy, and gas analysis revealed that the subsurface discontinuous cracks at the bore edges and in the fillet radius of the heat-treated end frame component had occurred due to hydrogen embrittlement, and not because of faulty heat treatment. This conclusion was supported by the presence of cracklike indications in machined bore surface of the annealed part.
SO2 Heat Exchanger Failure
Authors: Reitz W. 
Published: May 2019

Abstract
Critical heat exchanger components are usually manufactured from durable steels, such as stainless steel, which exhibit good strength and corrosion resistance. Failure of a heat exchanger occurred due to specification of a plain carbon steel that did not survive service in the SO2 vapor environment. However, failure analysis showed that cavitation erosion was the responsible failure mechanism, not corrosion as might be expected.